Continuous Cooling Transformation (CCT) Diagrams


 Heather Marshall
 2 years ago
 Views:
Transcription
1 Continuous Cooling Transformation (CCT) Diagrams R. Manna Assistant Professor Centre of Advanced Study Department of Metallurgical Engineering Institute of Technology, Banaras Hindu University Varanasi , India Tata SteelTRAERF Faculty Fellowship Visiting Scholar Department of Materials Science and Metallurgy University of Cambridge, Pembroke Street, Cambridge, CB2 3QZ
2 Continuous cooling transformation (CCT) diagram Definition: Stability of phases during continuous cooling of austenite There are two types of CCT diagrams I) Plot of (for each type of transformation) transformation start, specific fraction of transformation and transformation finish temperature against transformation time on each cooling curve II) Plot of (for each type of transformation) transformation start, specific fraction of transformation and transformation finish temperature against cooling rate or bar diameter for each type of cooling medium 2
3 Determination of CCT diagram type I CCT diagrams are determined by measuring some physical properties during continuous cooling. Normally these are specific volume and magnetic permeability. However, the majority of the work has been done through specific volume change by dilatometric method. This method is supplemented by metallography and hardness measurement. In dilatometry the test sample (Fig. 1) is austenitised in a specially designed furnace (Fig. 2) and then controlled cooled. Sample dilation is measured by dial gauge/sensor. Slowest cooling is controlled by furnace cooling but higher cooling rate can be controlled by gas quenching. 3
4 Fig. 1: Sample and fixtures for dilatometric measurements Fig. 2 : Dilatometer equipment 4
5 Temperature Dilation Cooling data are plotted as temperature versus time (Fig. 3). Dilation is recorded against temperature (Fig. 4). Any slope change indicates phase transformation. Fraction of transformation roughly can be calculated based on the dilation data as explained below. For a cooling schedule c X a I Time IV III II Fig. 3: Schematic cooling curves Y b V d Z T F Temperature T S Fig. 4: Dilationtemperature plot 5 for a cooling curve T
6 In Fig. 3 curves I to V indicate cooling curves at higher cooling rate to lower cooling rate respectively. Fig. 4 gives the dilation at different temperatures for a given cooling rate/schedule. In general slope of dilation curve remains unchanged while amount of phase or the relative amount of phases in a phase mixture does not change during cooling (or heating) however sample shrink or expand i.e. dilation takes place purely due to thermal specific volume change because of change in temperature. Therefore in Fig. 4 dilation from a to b is due to specific volume change of high temperature phase austenite. But at T S slope of the curve changes. Therefore transformation starts at T S. Again slope of the curve from c to d is constant but is different from the slope of the curve from a to b. This indicates there is no phase transformation between the temperature from c to d but the phase/phase mixture is different from the phase at a to b. 6
7 Slope of the dilation curve from b to c is variable with temperature. This indicates the change in relative amount of phase due to cooling. The expansion is due to the formation of low density phase(s). Some part of dilation is compensated by purely thermal change due to cooling. Therefore dilation curve takes complex shape. i.e first slope reduces and reaches to a minimum value and then increases to the characteristic value of the phase mixture at c. Therefore phase transformation start at b i.e. at temperature T S and transformation ends or finishes at c or temperature T F. The nature of transformation has to be determined by metallography. When austenite fully transforms to a single product then amount of transformation is directly proportional to the relative change in length. For a mixture of products the percentage of austenite transformed may not be strictly proportional to change in length, however, it is reasonable and generally is being used. 7
8 Cumulative percentage of transformation at in between temperature T is equal to YZ/XZ*100 where X, Y and Z are intersection point of temperature T line to extended constant slope curve of austenite (ba), transformation curve (bc) and extended constant slope curve of low temperature phase (cd) respectively. So at each cooling rate transformation start and finish temperature and transformation temperature for specific amount (10 %, 20%, 30% etc.) can also be determined. For every type of transformation, locus of start points, isopercentage points and finish points give the transformation start line, isopercentage lines and finish line respectively and that result CCT diagram. Normally at the end of each cooling curve hardness value of resultant product at room temperature and type of phases obtained are shown. 8
9 Fig. 5 shows the five different cooling curves a to e employed to a hypoeutectoid steel. Fig. 5(a) to (e) show the type of corresponding dilatometric plots drawn against dilation versus temperature. Fig. 6 shows the corresponding transformation temperature and time in a temperature versus log time plot against each corresponding cooling rate. At the end of each cooling rate curve normally hardness value and type of phases obtained at room temperature are shown. Symbols F, P, B, M stand for ferrite, pearlite, bainite and martensite respectively. Subscripts S and F stand for reaction start and reaction finish respectively. In cooling a schedule martensite starts at M S and finishes at M F and therefore 100% martensite results. While in cooling schedule b bainite starts at B S but reaction does not complete and retained austenite enriched in carbon transforms at lower M S but completes at lower M F. Cooling schedule b results bainite and martensite. 9
10 Dilation dilation Dilation dilation Temperature Temperature dilation M F F F F S a b c d e Time c B M S S Temperature Ae 3 Ae 1 F S a M F M S d B F F F B S F S a b c d e temperature Temperature Temperature Temperature M S B S P S M F b M S B S e P F P S F S M F B F M M+B F+B F+B F+P HV HV HV HV HV Log time Fig. 5: Schematic dilatometric plots for five different cooling rates where F, Fig. 6: Schematic CCT diagram constructed P, B and M stands for ferrite, pearlite, bainite and martensite respectively from data of Fig 3(for the hypoeutectoid and subscript S and F stands for transformation start and transformation steel). Dotted line is 25% of total finish for respective products for a hypoeutectoid steel transformation. 10
11 In cooling schedule c ferrite starts at F S and finishes at F F. Quantity of ferrite is about 15% but rest of austenite enriched in carbon transforms to bainite at B S and just finishes at B F. Therefore cooling c results ferrite and bainite at room temperature. Similarly cooling schedule d results increased ferrite and rest bainite. During cooling schedule e ferrite start at F S and pearlite starts at P S but pearlite reaction finishes at P F. Therefore cooling schedule e results increased ferrite and rest pearlite. The locus of all start points and finish points result the CCT diagram. This diagram is not a unique diagram like TTT diagram for a material. It depends on type of cooling. This diagram can predict phase transformation information if similar cooling curves had been used during its determination or if equivalent cooling schedule are used during process of production. 11
12 The two cooling curves are considered equivalent if (i) the times to cool from A e3 to 500 C are same. (ii) the times to cool from A e3 to a temperature halfway between Ae 3 and room temperature, are same. (iii) the cooling rates are same. (iv) the instant cooling rates at 700 C are same. Therefore to make it useful different types of CCT diagrams need to be made following any one of the above schedule that matches with heat treatment cooling schedule. 12
13 Endquench test method for type I CCT diagram A number of Jominy end quench samples are first end quenched (Fig.7) for a series of different times and then each of them (whole sample) is quenched by complete immersion in water to freeze the already transformed structures. Cooling curves are generated putting thermocouple at different locations and recording temperature against cooling time during end quenching. Microstructures at the point where cooling curves are known, are subsequently examined and measured by quantitative metallography. Hardness measurement is done at each investigated point. Based on metallographic information on investigated point the transformation start and finish temperature and time are determined. The transformation temperature and time are also determined for specific amount of transformation. These are located on cooling curves plotted in a temperature versus time diagram. The locus of transformation start, finish or specific percentage of transformation generate CCT diagram (Fig. 8). 13
14 1⅛ (29 mm) diameter ⅛ (3.2 mm) ½ (12.7 mm) 1⅓ 2 (26.2 mm) 2½ (64 mm) Free height of water jet Nozzle 1 (25.4 mm) diameter Water umbrella ½ (12.7 mm) ½ (12.7 mm) diameter 4 (102 mm) long Fig 7(a): Jominy sample with fixture and water jet 14
15 b c d Fig.7: Figures show (b) experimental set up, (c ) furnace for austenitisation, (d) end quenching process. Courtesy of DOITPoMS of Cambridge University. 15
16 Temperature Hardness, HRC A e1 F B A E D C Distance from quench end a b c d Jominy sample A t o =Minimum incubation period at the nose of the TTT diagram, t o =minimum incubation period at the nose of the CCT diagram t 0 t 0 B F E C D M S, Martensite start temperature M 50, 50% Martensite Metastable austenite +martensite M F, Martensite finish temperature Martensite Martensite Pearlite+Martensite Fine pearlite pearlite Coarse pearlite Log time Fig. 8: CCT diagram ( ) projected on TTT diagram ( ) of eutectoid steel 16
17 Fig. 7. shows the Jominy test set up and Fig. 6 shows a schematic CCT diagram. CCT diagram is projected on corresponding TTT diagram. A, B, C, D, E, F are six different locations on the Jominy sample shown at Fig.8 that gives six different cooling rates. The cooling rates A, B, C, D, E, F are in increasing order. The corresponding cooling curves are shown on the temperature log time plot. At the end of the cooling curve phases are shown at room temperature. Variation in hardness with distance from Jominy end is also shown in the diagram. For cooling curve B, at T 1 temperature minimum t 1 timing is required to nucleate pearlite as per TTT diagram in Fig. 8. But material has spent t 1 timing at higher than T 1 temperature in case of continuous cooling and incubation period at higher temperature is much more than t 1. The nucleation condition under continuous cooling can be explained by the concept of progressive nucleation theory of Scheil. 17
18 Scheil s concept of fractional nucleation/progressive nucleation Scheil presented a method for calculating the transformation temperature at which transformation begins during continuous cooling. The method considers that (1) continuous cooling occurs through a series of isothermal steps and the time spent at each of these steps depends on the rate of cooling. The difference between successive isothermal steps can be considered to approach zero. (2) The transformation at a temperature is not independent to cooling above it. (3) Incubation for the transformation occurs progressively as the steel cools and at each isothermal step the incubation of transformation can be expressed as the ratio of cooling time for the temperature interval to the incubation period given by TTT diagram. This ratio is called the fractional nucleation time. 18
19 Scheil and others suggested that the fractional nucleation time are additive and that transformation begins when the sum of such fractional nucleation time attains the value of unity. The criteria for transformation can be expressed Δt 1 /Z 1 +Δt 2 /Z 2 +Δt 3 /Z 3 +.+Δt n /Z n =1 Where Δt n is the time of isothermal hold at Temperature T n where incubation period is Z n. This is called additive reaction rule of Scheil (1935). The reactions for which the additive rule is justifiied are called isokinetic, implying that the fraction transform at any temperature depends only on time and a single function of temperature. This is experimentally verified by Krainer for pearlitic transformation. 19
20 Therefore though nucleation has progressed to some fraction of the event but time is not sufficient for pearlite nucleation at a. If time is allowed in continuous cooling while summation of fractional nucleation time becomes unity (at b), pearlite is to nucleate but by that time temperature drops down as it is continuously cooling. This concept of progressive nucleation is not strictly valid for bainite transformation where austenite get enriched with carbon at higher temperature. As transformation at higher temperature enriches the austenite by carbon, the transformation characteristic changes. i.e. transformation slows down at lower temperature. By continuous cooling transformation temperature moves towards down and incubation moves toward right. Similar is the case for pearlite finish temperature and time. Pearlitic region takes the shape as shown in the diagram. The bainitic region moves so right that entire region is sheltered by the pearlitic curve. 20
21 So there is no chance of bainitic tranformation in eutectoid plain carbon steel under continuous cooling condition. There is untransformed region where earlier was bainitic region. Under such circumtances split transformation occurs. However martensitic region remain unaffected. Various cooling rates give various combination of phases. Cooling A indicates very slow cooling rate equivalent to furnace cooling of full annealing process and that results coarse pearlite. Cooling B is faster cooling can be obtained by air cooling. This type of cooling can be obtained by normalising and that results finer pearlite. Cooling C: just touches the finishing end of nose that gives fully fine pearlite. Cooling D is faster cooling that can be obtained by oil quenching. This is a hardening heat treatment process and that produces fine pearlite and untransformed austenite transforms to martensite below M S. 21
22 Cooling curve E just touches the nose of CCT diagram and that produces almost fully martensite. Cooling curve F avoid nose of C curve in CCT but touches the nose of TTT gives entirely martensite. Notice the critical cooling rate to avoid nose of CCT diagram i.e. diffusional transformations is lower than that to TTT diagram. 22
23 General features of CCT diagrams 1. CCT diagram depends on composition of steel, nature of cooling, austenite grain size, extent of austenite homogenising, as well as austenitising temperature and time. 2. Similar to TTT diagrams there are different regions for different transformation (i.e. cementite/ferrite, pearlite, bainite and martensite). There are transformation start and transformation finish line and isopercentage lines. However depending on factors mentioned earlier some of the transformation may be absent or some transformation may be incomplete. 3. In general for ferrite, pearlite and bainite transformation start and finish temperature moves towards lower temperature and transformation time towards higher timing in comparison to isothermal transformation. Transformation curve moves down and right. 23
24 4. The bainite reaction can be sufficiently retarded such that transformation takes shelter completely under pearlitic transformation in case of eutectoid plain carbon steel and therefore bainite region vanishes. However in other steel it may be partially sheltered. Therefore bainitic region observed in non eutectoid plain carbon steel or alloy steels. 5. C curves nose move to lower temperature and longer time. So actual critical cooling rate required to avoid diffusional transformation during continuous cooling is less than as prescribed by TTT diagram. Actual hardenability is higher than that predicted by TTT. 6. M S temperature is unaffected by the conventional cooling rate,however, it can be lowered at lower cooling rate if cooling curves such that austenite enriches with carbon due to bainite or ferrite formation (in hypoeutectoid steel). On the other hand M S can go up for lower cooling rate such that austenite become lean in carbon due to carbide separation (in hypereutectiod steel). 24
25 7. Large variety of microstructure like ferrite/cementite/carbide +pearlite+bainite+martensite can be obtained in suitable cooling rate. It is not feasible or limited in case of isothermal transformation. 25
26 Determination of type II CCT diagram This procedure was developed by Atkins. In this process round samples of different diameters were quenched in three different media air, oil and water. The cooling curves were recorded at the centre of each bar. Later these cooling curves were simulated in dilatometer test in order to identify the transformation temperature, microstructure and hardness. The transformation information is plotted against temperature and bar diameter cooled in specific medium. These are bar diameter cooled in air, quenched in oil and quenched in water. A scale cooling rate (usually at 700 C) in C/min is added. At the bottom of the same diagram another plot is added for hardness (in HRC) and with same cooling rate axis/bardiameter. These diagrams have to be read along vertical lines (from top to bottom), denoting different cooling rates. Fig. 9 shows a schematic CCT diagram for hypoeutectoid plain carbon steel. 26
27 Hardness, HV Hardness, HRC Temperature, C 0% 50% 90% 100% M s Fig. 9: CCT diagram for hypoeutectoid steel M 50 M 90 M f Cooling rate at 700 C, C per min Bar diameter, in mm Oil quench Water quench Air cooled Hardness after transformation at room temperature 27
28 Conversion of TTT to CCT diagram, Scheil s method (1935) Scheil s method is based on the assumption that the continuous cooling curve is a combination of sufficiently large number of isothermal reaction steps. Incubation for the transformation occurs progressively as the steel continuously cools. Transformation begins when the sum of fractional nucleation time attains the value of unity. The criteria for transformation can be expressed Δt 1 /Z 1 +Δt 2 /Z 2 +Δt 3 /Z 3 +.+Δt n /Z n =1 Where Δt n is the time of isothermal hold at temperature T n where incubation period is Z n. The rule can be justified if reaction rate solely depends on volume fraction and temperature. 28
29 Conversion of TTT to CCT, Grange and Kiefer Method (1941) During continuous cooling along a given cooling curve which intercepts the TTT start curve at temperature T 1, the transformation will start at temperature T 2, such that the time of cooling between T 1 and T 2 is equal to the time for the start of transformation during isothermal holding at temperature T 3 = (T 1 +T 2 )/2 (as shown in Fig. 10). t 3 =t 2 t 1 Similar rule can be applied for a isopercentage curve and finish curves. Assumptions are not strictly valid, however, the method gives reasonable result. The method is particularly suitable for ferritepearlite region 29
30 Temperature Ae 3 T 1 T 3 T 2 T 3 =(T 1 +T 2 )/2 and t 3 =t 2 t 1 or t 2 =(t 1 +t 3 )/2 t 3 t 1 t 2 Log time Fig. 10: Graphic method of converting TTT diagram to CCT diagram [Grange and Kiefer method] 30
31 Conversion of TTT to CCT, Avrami method (1939) Let τ TTT (T) be time required to obtain a given percentage of transformation, X at temperature T during isothermal transformation. Then time required(τ CCT ) to obtain the same percentage of transformation, X, on continuous cooling at T CCT is given by the condition X= T Ae 3 CCT dx= T CCT Ae dx/dt.dt= T CCT g 3 Ae dt g=time average transformation rate (at any temperature T)=X/τ IT (T). Substituting this in equation 1 We get Ae 3T CCT dt/ τ TTT (T) = , By rewriting equation 2 we get Ae 3T CCT dt/(τ TTT (T) dt/dt)= Both these integrals are called Avrami integral. Any one of these integrals has to be evaluated for each cooling curve to get the τ CCT at T CCT 31
32 Conversion of CCT to TTT diagram, Kirkaldy and Sharma method (1982) Let τ CCT (T CCT ) be the time required to obtain a given percentage of transformation, X at temperature T CCT during continuous cooling. If it is assumed that CCT diagram was constructed using constant cooling rate(linear cooling), Then dt/dt=(a e3 T CCT )/(τ CCT (T CCT )4 Substituting equation 4 in equation 3, cross multiplying and differentiating with respect to T CCT We get τ TTT (T CCT )=1/(d/dT CCT [(A e3 T CCT )/τ CCT (T CCT )])5 Where τ TTT is the time required for the given percentage transformation, X, when carried out isothermally at T CCT. 32
33 While rate of cooling is not constant but cooling rate can be expressed analytically or empirically as dt/dt=f 1 (x)f 2 (T)=f 1 (T CCT )f 2 (T) 6 curve can be expressed in this form) (Exp: Jominy cooling where x is the distance from the surface of a continuouly cooled sample. Substituting equation 6 in equation 3, cross multiplying and differentiating We get τ TTT (T CCT )=1/(f 2 (T CCT ) df 1 /dt CCT ) Equation 5 or 7 can be used for the conversion of CCT diagram to TTT diagram depending on constant cooling rate or case of cooling rate that can be expressed in analytical or empirical form. Jominy cooling curves can be expressed in equation 6 form and the using equation 7, CCT diagram can be converted to TTT diagram. 33
Solution: ΔG = a 3 ΔG v. + 6a 2 γ. Differentiation of this expression with respect to a is as. d ΔG da = d(a3 ΔG v. + d(6a2 γ) = 3a 2 ΔG v.
14:440:407 ch10 Question 10.2: (a) Rewrite the expression for the total free energy change for nucleation (Equation 10.1) for the case of a cubic nucleus of edge length a (instead of a sphere of radius
More information5 Some standard heat treatments
Part VI. : Heat treatment Module 5 : Some standard heat treatments 5 Some standard heat treatments 5.1 Annealing Consider the TTT diagram as shown in Fig. 9 and the cooling curves imposed on the TTT diagram.
More informationChapter Outline: Phase Transformations in Metals
Chapter Outline: Phase Transformations in Metals Heat Treatment (time and temperature) Microstructure Mechanical Properties Kinetics of phase transformations Multiphase Transformations Phase transformations
More informationIronCarbon Phase Diagram (a review) see Callister Chapter 9
IronCarbon Phase Diagram (a review) see Callister Chapter 9 University of Tennessee, Dept. of Materials Science and Engineering 1 The Iron Iron Carbide (Fe Fe 3 C) Phase Diagram In their simplest form,
More informationHeat Treatment of Steels : Spheroidize annealing. Heat Treatment of Steels : Normalizing
Heat Treatment of Steels :Recrystallization annealing The carbon and alloy steels were treated at a temperature of about 700 C, which is about 20 C below the eutectoid temperature. The holding time should
More informationSection 3: HEAT TREATMENT
Section 3: HEAT TREATMENT Introduction Objectives of Heat Treatment Heat Treatment is the controlled heating and cooling of metals to alter their physical and mechanical properties without changing the
More informationExperiment: Heat Treatment  Quenching & Tempering
Experiment: Heat Treatment  Quenching & Tempering Objectives 1) To investigate the conventional heat treatment procedures, such as quenching and annealing, used to alter the properties of steels. SAE
More informationDr. Pulak M. Pandey. paniit.iitd.ac.in/ ~ pmpandey
Dr. Pulak M. Pandey http:// paniit.iitd.ac.in/ ~ pmpandey Metals and alloys may not posses all the desired properties in the finished product. Alloying and heat treatment are two methods which are extensively
More informationModule 34. Heat Treatment of steel IV. Lecture 34. Heat Treatment of steel IV
Module 34 Heat reatment of steel IV Lecture 34 Heat reatment of steel IV 1 Keywords : Austenitization of hypo & hyper eutectoid steel, austenization temperature, effect of heat treatment on structure &
More informationHeat Treatment of Steel
Heat Treatment of Steel Steels can be heat treated to produce a great variety of microstructures and properties. Generally, heat treatment uses phase transformation during heating and cooling to change
More informationModule 4 Design for Assembly IIT BOMBAY
Module 4 Design for Assembly Lecture Design for Heat Treatment 7 Instructional objectives By the end of this lecture, the student will learn 1. different heat treatment processes, 2. application of various
More informationEVALUATION METHODS OF DILATOMETER CURVES OF PHASE TRANSFORMATIONS
EVALUATION METHODS OF DILATOMETER CURVES OF PHASE TRANSFORMATIONS Petr MOTYČKA 1, Michal KÖVÉR 1,2 1 COMTES FHT a.s., Průmyslová 995, Dobřany, Czech Republic, 2 Slovak University of Technology in Bratislava,
More informationTime Temperature Transformation (TTT) Diagrams
Tata SteelTRAERF Faculty Fellowship Visiting Scholar Department of Materials Science and Metallurgy University of Cambridge, Pembroke Street, Cambridge, CB2 3QZ rm659@cam.ac.uk Time Temperature Transformation
More informationHEAT TREATMENT OF STEEL
HEAT TREATMENT OF STEEL Heat Treatment of Steel Most heat treating operations begin with heating the alloy into the austenitic phase field to dissolve the carbide in the iron. Steel heat treating practice
More informationLABORATORY EXPERIMENTS TESTING OF MATERIALS
LABORATORY EXPERIMENTS TESTING OF MATERIALS 1. TENSION TEST: INTRODUCTION & THEORY The tension test is the most commonly used method to evaluate the mechanical properties of metals. Its main objective
More informationIntroduction to Iron Metallurgy. Lee Morin Houston Home Metal Shop Club October 2010
Introduction to Iron Metallurgy Lee Morin Houston Home Metal Shop Club October 2010 Book I stole the pictures from We will start with a brief overview! Metals Are Crystals Fundamental geometry of a crystal
More informationCHROMIUM STEEL POWDERS FOR COMPONENTS. JEANETTE LEWENHAGEN Höganäs AB, Sweden
CHROMIUM STEEL POWDERS FOR COMPONENTS JEANETTE LEWENHAGEN Höganäs AB, Sweden KEYWORDS Prealloyed steel powder, chromium, PM ABSTRACT Chromium as an alloying element is of great interest due to its low
More informationIntroduction to Materials Science, Chapter 11, Thermal Processing of Metal Alloys. Chapter 11 Thermal Processing of Metal Alloys
Chapter 11 Thermal Processing of Metal Alloys Designer Alloys: Utilize heat treatments to design optimum microstructures and mechanical properties (strength, ductility, hardness.) Strength in steels correlates
More informationMATERIALS 101 INTRODUCTION TO STRUCTURE AND PROPERTIES WINTER Problem Set 6 Due: Tuesday, March 6, 11:00 AM
Problem Set 6 Due: Tuesday, March 6, 11:00 AM 1. TTT Diagrams Based on the transformation diagrams for eutectoid steel shown below, what microstructure would result from the following cooling histories?
More informationThe atomic packing factor is defined as the ratio of sphere volume to the total unit cell volume, or APF = V S V C. = 2(sphere volume) = 2 = V C = 4R
3.5 Show that the atomic packing factor for BCC is 0.68. The atomic packing factor is defined as the ratio of sphere volume to the total unit cell volume, or APF = V S V C Since there are two spheres associated
More informationINFLUENCE OF THERMOMECHANICAL TREATMENT ON THE STEEL C45 FATIGUE PROPERTIES
COMATTECH 2005 TRNAVA, 2021 October 2005 INFLUENCE OF THERMOMECHANICAL TREATMENT ON THE STEEL C45 FATIGUE PROPERTIES Jiří MALINA 1+2, Hana STANKOVÁ 1+2, Jaroslav DRNEK 3, Zbyšek NOVÝ 3, Bohuslav MAŠEK
More informationAlloys & Their Phase Diagrams
Alloys & Their Phase Diagrams Objectives of the class Gibbs phase rule Introduction to phase diagram Practice phase diagram Lever rule Important Observation: One question in the midterm Consider the Earth
More informationUniversity of Cambridge, Materials Science & Metallurgy. Dilatometry
University of Cambridge, Materials Science & Metallurgy H. K. D. H. Bhadeshia Dilatometry The dilatometric method utilises either transformation strains or thermal strains; the basic data generated are
More informationLecture 19: Eutectoid Transformation in Steels: a typical case of Cellular
Lecture 19: Eutectoid Transformation in Steels: a typical case of Cellular Precipitation Today s topics Understanding of Cellular transformation (or precipitation): when applied to phase transformation
More informationComposition Solidus Liquidus (wt% Au) Temperature ( C) Temperature ( C)
10.4 Given here are the solidus and liquidus temperatures for the copper gold system. Construct the phase diagram for this system and label each region. Composition Solidus Liquidus (wt% Au) Temperature
More informationEffect of Heat Treatment on the Microstructure and Mechanical Properties of Steel
金属材料及热处理 学生实验报告范例课程编号 :030107 课程主讲及实验课指导教师 : 刘国权黄鹏 Effect of Heat Treatment on the Microstructure and Mechanical Properties of Steel Song Zhen 40531165 University of Science and Technology Beijing, Dept.of
More informationCarbon Equivalent to Assess Hardenability of Steel and Prediction of HAZ Hardness Distribution
UDC 621. 791. 053 : 539. 531 : 669. 784 Carbon Equivalent to Assess Hardenability of Steel and Prediction of HAZ Hardness Distribution Tadashi KASUYA* 1 Yuji HASHIBA* 1 Abstract A practical method to predict
More informationPOSSIBILITY OF INDIRECT HARDNESS TESTING OF DUPLEX STAINLESS STEEL
1 POSSIBILITY OF INDIRECT HARDNESS TESTING OF DUPLEX STAINLESS STEEL István Mészáros Associate professor, Department of Materials Science and Engineering H1111 Budapest, Goldmann tér 3. Summary In this
More informationX15TN TM. A high hardness, corrosion and fatigue resistance martensitic grade CONTINUOUS INNOVATION RESEARCH SERVICE.
TM A high hardness, corrosion and fatigue resistance martensitic grade CONTINUOUS METALLURGICAL SPECIAL STEELS INNOVATION RESEARCH SERVICE DEVELOPMENT Enhancing your performance THE INDUSTRIAL ENVIRONMENT
More informationProblem Set 7 Materials101 1.) You wish to develop a gold alloy (mostly gold) that can be precipitation strengthened to provide high strength  high conductivity electrical leads to integrated circuits
More informationEffect of Heat Treatment Processes on the Mechanical Properties of Medium Carbon Steel
Journal of Minerals & Materials Characterization & Engineering, Vol. 11, No.2 pp.143152, 2012 jmmce.org Printed in the USA. All rights reserved Effect of Heat Treatment Processes on the Mechanical Properties
More information= 62 wt% Ni38 wt% Cu.
92 9.2 (a) From Figure 9.8, the maximum solubility of Pb in Sn at 100 C corresponds to the position of the β (α + β) phase boundary at this temperature, or to about 2 wt% Pb. (b) From this same figure,
More informationDevelopment of HighStrength Steel Wire with Superior Weldability
INDUSTRIAL MATERIALS Development of HighStrength Steel Wire with Superior Weldability Hiromu IzumIda*, Kenichi SHImIzu, Shinei TaKamura, Yasuhiro SHImoda, osamu momozawa and Teruyuki murai Highcarbon
More informationChapter 10: Phase Transformations
Chapter 10: Phase Transformations ISSUES TO ADDRESS... Transforming one phase into another takes time. Fe C FCC γ (Austenite) Eutectoid transformation Fe 3 C (cementite) + α (ferrite) (BCC) How does the
More informationThe mechanical properties of metal affected by heat treatment are:
Training Objective After watching this video and reviewing the printed material, the student/trainee will learn the basic concepts of the heat treating processes as they pertain to carbon and alloy steels.
More informationHigh carbon and quenchable steels Hot Rolled Steel Plate and Coil for Hardening and Wear Resistance
Data Sheet: A2.2 High carbon and quenchable steels Hot Rolled Steel Plate and Coil for Hardening and Wear Resistance General description Steel is generally classified as high carbon steel if the nominal
More informationAustempering Heat Treatment of AISI 4340 Steel and Comparative Analysis of Various Physical Properties at Different Parameters
Austempering Heat Treatment of AISI 4340 Steel and Comparative Analysis of Various Physical Properties at Different Parameters Najeeb Niazi 1,*, Salman Nisar 1 and Aqueel Shah 1 1 Department of Manufacturing
More informationGrade C Si Mn Cr Mo V RWL34 1,05 0,50 0, ,2
Martensitic stainless RWL 34 Damasteel s martensitic stainless RWL 34 is a Rapid Solidified Powder (RSP) based steel which is a variation of the 420 martensitic stainless steel with > 13 % Chromium. The
More informationSimulations of the Effect of Section Size and Cooling on Sigma Phase Formation in Duplex Stainless Steels
Simulations of the Effect of Section Size and Cooling on Sigma Phase Formation in Duplex Stainless Steels Richard A. Hardin and Christoph Beckermann Department of Mechanical and Industrial Engineering
More informationPhase Transformations in Metals and Alloys
Phase Transformations in Metals and Alloys THIRD EDITION DAVID A. PORTER, KENNETH E. EASTERLING, and MOHAMED Y. SHERIF ( г йс) CRC Press ^ ^ ) Taylor & Francis Group Boca Raton London New York CRC Press
More informationImproved Broaching Steel Technology
Improved Broaching Steel Technology Michael E. Burnett TimkenSteel Corporation 1835 Dueber Ave. SW, Canton Ohio 44706 Phone: (330) 4713273 Email: michael.burnett@timkensteel.com Key Words: Alloy Steel,
More informationFundamentals of the Heat Treating of Steel
CHAPTER 2 Fundamentals of the Heat Treating of Steel BEFORE CONSIDERATION can be given to the heat treatment of steel or other ironbase alloys, it is helpful to explain what steel is. The common dictionary
More informationEffect of Heat Treatment on Mechanical Properties and Microstructure of NST 372 Steel
Journal of Minerals & Materials Characterization & Engineering, Vol. 10, No.3, pp.299308, 2011 jmmce.org Printed in the USA. All rights reserved Effect of Heat Treatment on Mechanical Properties and Microstructure
More informationHIGH STRENGTH DUCTILE IRON PRODUCED BY THE ENGINEERED COOLING: PROCESS CONCEPT
IJMC142442 HIGH STRENGTH DUCTILE IRON PRODUCED BY THE ENGINEERED COOLING: PROCESS CONCEPT Copyright 215 American Foundry Society Abstract Simon N. Lekakh Missouri University of Science and Technology,
More informationHeat Transfer Coefficients during Quenching of Steels
Noname manuscript No. (will be inserted by the editor) Heat Transfer Coefficients during Quenching of Steels H. S. Hasan M. J. Peet J. M. Jalil H. K. D. H. Bhadeshia Received: date / Accepted: date Abstract
More informationHW 8. G = a 3 G v. 6a 2. Problem a. To Find:
HW 8 Problem 10. a. To Find: (a) The expression for total free energy change for a cubic nucleus, critical cube edge length, a*, and G* (b) Compare G* for a cube with that for a sphere b. Given: Nucleus
More informationChapter 1 Introduction to Material science & Metallurgy
Chapter 1 Introduction to Material science & Metallurgy 1. Material Science & Metallurgy (21419) State the importance of study of materials science and briefly. Explain Engineering requirements of materials.
More informationMaterial Science Engineering and Steel Making/Metallurgy. Stark County High Schools 2016
Material Science Engineering and Steel Making/Metallurgy Stark County High Schools 2016 Agenda What is Material Science Engineering Basics of Steel Making Steel Processing and Properties 2 What is Material
More informationVacuum heat treatment and high pressure gas quenching Aspects in Distortion Control
HEAT TREATMENT REPORTS Vacuum heat treatment and high pressure gas quenching Aspects in Distortion Control Jean Jaques Since, Olaf Irretier L This technical article reviews high pressure gas quenching
More information3. Apply phase rule to the two phase field of a binary isomorphous diagram. What conclusion can be drawn?
ecture 1822: Solidification of binary alloys: Solidification of binary alloys: limits of solubility, isomorphous system, lever rule, constitutional super cooling, effect of non equilibrium cooling, eutectic,
More informationEffect of Heat Treatment Process on the Fatigue Behavior of AISI 1060 Steel
International International Journal of ISSI, Journal Vol. of 12 ISSI, (2015), Vol.10 No.1, (2013), pp. 2832 No.1 Effect of Heat Treatment Process on the Fatigue Behavior of AISI 1060 Steel M. Mehdinia
More informationDamasteel s martensitic stainless Nitrobe 77 is a powder based steel which solves two classical knife problems:
Damasteel s martensitic stainless Nitrobe 77 is a powder based steel which solves two classical knife problems: Sharp edges on chef knives. Nitrobe 77 is dishwasher safe without risk of corrosion or edge
More informationDevelopment of a High Performance NickelFree P/M Steel. Bruce Lindsley. Senior Materials Engineer, Hoeganaes Corporation, Cinnaminson, NJ 08077, USA
Development of a High Performance NickelFree P/M Steel Bruce Lindsley Senior Materials Engineer, Hoeganaes Corporation, Cinnaminson, NJ 08077, USA Abstract A developmental nickelfree P/M steel containing
More informationLife Management Technique of Thermal Fatigue for SMST Boiler Tube at Different Heating Zone Using Smithy Furnace
RESEARCH ARTICLE OPEN ACCESS Life Management Technique of Thermal Fatigue for SMST Boiler Tube at Different Heating Zone Using Smithy Furnace Shekhar Pal, Pradeep Suman, Shri dk jain.gpc kota MTech in
More informationIntroduction of Materials Modelling into Processing Simulation Towards True Virtual Design and Simulation
International Journal of Metallurgical Engineering 2013, 2(2): 198202 DOI: 10.5923/j.ijmee.20130202.11 Introduction of Materials Modelling into Processing Simulation Towards True Virtual Design and Simulation
More informationWHAT IS SINTERHARDENING? W. Brian James. Hoeganaes Corporation Cinnaminson, NJ 08077
WHAT IS SINTERHARDENING? W. Brian James Abstract Hoeganaes Corporation Cinnaminson, NJ 08077 Presented at PM 2 TEC '98 International Conference on Powder Metallurgy & Particulate Materials May 31  June
More informationDevelopment of API X80 Grade Electric Resistance Welding Line Pipe with Excellent Low Temperature Toughness
JFE TECHNICAL REPORT No. 12 (Oct. 2008) Development of API X80 Grade Electric Resistance Welding Line Pipe with Excellent Low Temperature Toughness NAKATA Hiroshi *1 KAMI Chikara *2 MATHUO Nobuyuki *3
More informationINFLUENCE OF Cr, Mn AND Mo ON STRUCTURE AND PROPERTIES OF V MICROALLOYED MEDIUM CARBON FORGING STEELS
Association of Metallurgical Engineers of Serbia AMES Scientific paper UDC: 669.15'26'74'28194 INFLUENCE OF Cr, Mn AND Mo ON STRUCTURE AND PROPERTIES OF V MICROALLOYED MEDIUM CARBON FORGING STEELS Nenad
More informationContinuous Cooling Bainite Transformation Characteristics of a Low Carbon Microalloyed Steel under the Simulated Welding Thermal Cycle Process
Available online at SciVerse ScienceDirect J. Mater. Sci. Technol., 2013, 29(5), 446e450 Continuous Cooling Bainite Transformation Characteristics of a Low Carbon Microalloyed Steel under the Simulated
More informationMARTENSITIC STAINLESS STEEL RWL34
MARTENSITIC STAINLESS STEEL RWL34 RWL 34 is a Rapid Solidified Powder (RSP) Martensitic Stainless Steel, which is variation of the 420 martensitic stainless steel family with minimum 13 percent chromium
More informationVACUUMHEATTREATMENT OF HOTWORK STEEL
VACUUMHEATTREATMENT OF HOTWORK STEEL B. Zieger SCHMETZ GmbH, Holzener Str. 39, 58708 Menden, Germany Abstract The heattreatment of tool and hotworking steels in horizontal vacuum furnaces is today
More informationTHREE MAIN SOLIDIFICATION REACTIONS OF VANADIUM MODIFIED T1 TUNGSTEN HIGH SPEED TOOL STEEL. Hossam Halfa
THREE MAIN SOLIDIFICATION REACTIONS OF VANADIUM MODIFIED T1 TUNGSTEN HIGH SPEED TOOL STEEL Hossam Halfa Steel Technology Department, Central Metallurgical R&D Institute (CMRDI), Helwan, Egypt, hossamhalfa@cmrdi.sci.eg;
More informationFull Density Properties of Low Alloy Steels
Full Density Properties of Low Alloy Steels Michael L. Marucci & Arthur J. Rawlings Hoeganaes Corporation, Cinnaminson, NJ Presented at PM 2 TEC2005 International Conference on Powder Metallurgy and Particulate
More informationHEAT TREATMENT PROCEDURE QUALIFICATION. Final Technical Report. The Pennsylvania State University University Park, PA
HEAT TREATMENT PROCEDURE QUALIFICATION Final Technical Report The Pennsylvania State University University Park, PA Work Performed Under Contract No. DEFC0799ID13841 Work Prepared for U.S. Department
More information8. Technical Heat Treatment
8. Technical Heat Treatment 8. Technical Heat Treatment 95 6 cm 4 2 02 4 C 400 C C 614 1210 86 42 0 2 cm 6 723 C temperature C 1750 750 250 When welding a workpiece, not only the weld itself,
More informationSimulation of Residual Stresses in an Induction Hardened Roll
2.6.4 Simulation of Residual Stresses in an Induction Hardened Roll Ludwig Hellenthal, Clemens Groth Walzen Irle GmbH, NetphenDeuz, Germany CADFEM GmbH, Burgdorf/Hannover, Germany Summary A heat treatment
More informationIn order to solve this problem it is first necessary to use Equation 5.5: x 2 Dt. = 1 erf. = 1.30, and x = 2 mm = 2 103 m. Thus,
5.3 (a) Compare interstitial and vacancy atomic mechanisms for diffusion. (b) Cite two reasons why interstitial diffusion is normally more rapid than vacancy diffusion. Solution (a) With vacancy diffusion,
More information9.11 Upon heating a leadtin alloy of composition 30 wt% Sn70 wt% Pb from 150 C and utilizing Figure
913 9.8: 9.11 Upon heating a leadtin alloy of composition 30 wt% Sn70 wt% Pb from 150 C and utilizing Figure (a) The first liquid forms at the temperature at which a vertical line at this composition
More informationSteel and cast iron. Chapter Chapter 112
Steel and cast iron Chapter 111 Chapter 112 1 Taxonomy of Metals Metal Alloys Ferrous Steels Cast Irons
More informationHeat treatment of steel parts in different media
Journal of Metals, Materials and Minerals, Vol.23 No.2 pp.17, 2013 Heat treatment of steel parts in different media Suresh C. MAIDARGI and Veena RANI* Department of Chemical Engineering, Dayananda Sagar
More informationQuality and Process Optimization of the Heat Treatment
Controlled Diffusion: Quality and Process Optimization of the Heat Treatment Summary of the innovative and adaptive control technology for the automatic creation of optimized treatment programs for diffusion
More informationUnderstanding Boiling Water Heat Transfer in Metallurgical Operations
Understanding Boiling Water Heat Transfer in Metallurgical Operations Dr. Mary A. Wells Associate Professor Department of Mechanical and Mechatronics Engineering University of Waterloo Microstructural
More information3. APPLICATION OF PLASMA FOR HEAT TREATMENT
3. APPLICATION OF PLASMA FOR HEAT TREATMENT Classification of chapters: 3.1. Plasma 3.2. Physical metallurgical characteristics of quenched surface zone 3.2.1. Factors influencing achieved properties of
More information4 Thermomechanical Analysis (TMA)
172 4 Thermomechanical Analysis 4 Thermomechanical Analysis (TMA) 4.1 Principles of TMA 4.1.1 Introduction A dilatometer is used to determine the linear thermal expansion of a solid as a function of temperature.
More informationEffect of Small Additions of Boron on the Mechanical Properties and Hardenability of Sintered P/M Steels
Effect of Small Additions of Boron on the Mechanical Properties and Hardenability of Sintered P/M Steels Michael Marucci *, Alan Lawley **, Robert Causton *, and Suleyman Saritas *** * Hoeganaes Corporation,
More informationAPI X80 Grade Electric Resistance Welded Pipe with Excellent Low Temperature Toughness
API X80 Grade Electric Resistance Welded Pipe with Excellent Low Temperature Toughness JFE TECHNICAL REPORT No. 18 (Mar. 2013) NAKATA Hiroshi *1 KAMI Chikara *2 MATSUO Nobuyuki *3 Abstract: This paper
More informationEstimating the Eutectic Composition of Simple Binary Alloy System Using Linear Geometry
Estimating the Eutectic Composition of Simple Binary Alloy System Using Linear Geometry Muhammed Olawale Hakeem AMUDA * and Raymond Otito AKABEKWA Department of Metallurgical and Materials Engineering
More informationSection 4: NiResist Iron
Section 4: NiResist Iron Section 4 NiResist Description of Grades...42 201 (Type 1) NiResist...43 202 (Type 2) NiResist...46 Stock Listings...48 41 NiResist Description of Grades NiResist DuraBar
More informationEFFECT OF COPPER ALLOY ADDITION METHOD ON THE DIMENSIONAL RESPONSE OF SINTERED FECUC STEELS
EFFECT OF COPPER ALLOY ADDITION METHOD ON THE DIMENSIONAL RESPONSE OF SINTERED FECUC STEELS Michael L. Marucci and Francis G. Hanejko Hoeganaes Corporation Cinnaminson, NJ 08077  USA Abstract FeCuC
More informationReservoir Fluids PETE 310
Reservoir Fluids PETE 31 Lab 2: Determination of the Vapor Pressure of Propane Learning Objectives When you complete this laboratory, you should be able to: Use closedcell and sightglass methods for
More informationINDUCTION WELDED SMALL DIAMETER TUBE PRODUCTION LINE
INDUCTION WELDED SMALL DIAMETER TUBE PRODUCTION LINE Target Production of welded single  wall tubing manufactured to ASTM A 513, also zinc coated as per UNI 574166, suitable for many low pressure and
More informationNorth American Stainless
Introduction: North American Stainless Flat Products Stainless Steel Grade Sheet 309S (S30908)/ EN1.4833 SS309 is a highly alloyed austenitic stainless steel used for its excellent oxidation resistance,
More informationTHE INVESTIGATION OF APPLICABILITY OF THE HOLLOMONJAFFE EQUATION ON TEMPERING THE HSLA STEEL
Available on line at Association of the Chemical Engineers AChE www.ache.org.rs/ciceq Chemical Industry & Chemical Engineering Quarterly 15 (3) 131 136 (2009) CI&CEQ ZORAN JANJUŠEVIĆ ZVONKO GULIŠIJA MARIJA
More informationComparison of Three NiHard I Alloys
Comparison of Three NiHard I Alloys Ö. N. Do an 1, J.A. Hawk 1, and J.Rice 2 1 U.S. Department of Energy, Albany Research Center, Albany, Oregon 2 Texaloy Foundry Co., Inc., Floresville, Texas Keywords:
More information6.2 Determination of Heats of Reaction
162 6 Applications of Differential Scanning Calorimetry 6.2 Determination of Heats of Reaction The aim is to determine a thermodynamically well defined (temperature dependent) reaction enthalpy. If a subsequent
More informationFATIGUE BEHAVIOUR ANALYSIS OF DIFFERENTLY HEAT TREATED MEDIUM CARBON STEEL. Master of Technology (Res.) Metallurgical and Materials Engineering
FATIGUE BEHAVIOUR ANALYSIS OF DIFFERENTLY HEAT TREATED MEDIUM CARBON STEEL A THESIS SUBMITTED IN PARTIAL FULFILLMENT OF THE REQUIREMENTS FOR THE DEGREE OF Master of Technology (Res.) in Metallurgical and
More informationDH31EX!!! NADCA Approved 2011
DH31EX!!! NADCA Approved 2011 Ultra High Strength, tough, and high heat check resistance hot work die steel. DH31EX, produced exclusively by Diado Steel Ltd., is a hot working die steel with the best
More informationTypes 410, 420, 425 Mod, and 440A
s 410, 420, 425 Mod, and 440A GENERAL PROPERTIES s 410, 420, 425 Modified, and 440A (see composition on Page 2) are hardenable, straightchromium stainless steels which combine superior wear resistance
More informationIntroduction to Materials Science, Chapter 9, Phase Diagrams. Phase Diagrams. University of Tennessee, Dept. of Materials Science and Engineering 1
Phase Diagrams University of Tennessee, Dept. of Materials Science and Engineering 1 Chapter Outline: Phase Diagrams Microstructure and Phase Transformations in Multicomponent Systems Definitions and basic
More informationCHAPTER 11 APPLICATIONS AND PROCESSING OF METAL ALLOYS PROBLEM SOLUTIONS
111 CHAPTER 11 APPLICATIONS AND PROCESSING OF METAL ALLOYS PROBLEM SOLUTIONS Ferrous Alloys 11.1 This question asks that we list four classifications of steels, and, for each, to describe properties and
More informationThe First Law of Thermodynamics: Closed Systems. Heat Transfer
The First Law of Thermodynamics: Closed Systems The first law of thermodynamics can be simply stated as follows: during an interaction between a system and its surroundings, the amount of energy gained
More informationATI 410 /ATI 420 /ATI 425 Mod / ATI 440A /ATI 440C
ATI 410 /ATI 420 /ATI 425 Mod / Stainless Steel: Martensitic (UNS S41000/S42000/xxxxx/S44002/S44004) GENERAL PROPERTIES ATI 410, ATI 420, ATI 425 Modified, and ATI 440A alloys (see composition on Page
More informationEffect of Prior Athermal Martensite on the Isothermal Transformation Kinetics Below M s in a LowC HighSi Steel
Effect of Prior Athermal Martensite on the Isothermal Transformation Kinetics Below M s in a LowC HighSi Steel A. NAVARROLO PEZ, J. SIETSMA, and M.J. SANTOFIMIA Thermomechanical processing of Advanced
More informationWELDING AND COATING METALLURGY
WELDING AND COATING METALLURGY 1 INTRODUCTION 4 1.1 ROLE OF CARBON IN STEEL 4 1.2 WELDABILITY OF STEELS 5 2 CRYSTAL STRUCTURE 7 2.1 SOLUBILITY OF CARBON 8 3 IRON  IRON CARBIDE PHASE DIAGRAM 9 3.1 AUSTENITE
More informationUDDEHOLM VANADIS 30 SUPERCLEAN
UDDEHOLM VANADIS 30 SUPERCLEAN UDDEHOLMS AB No part of this publication may be reproduced or transmitted for commercial purposes without permission of the copyright holder. This information is based on
More informationSolution for Homework #1
Solution for Homework #1 Chapter 2: Multiple Choice Questions (2.5, 2.6, 2.8, 2.11) 2.5 Which of the following bond types are classified as primary bonds (more than one)? (a) covalent bonding, (b) hydrogen
More informationInteractive Math Glossary Terms and Definitions
Terms and Definitions Absolute Value the magnitude of a number, or the distance from 0 on a real number line Additive Property of Area the process of finding an the area of a shape by totaling the areas
More informationInduction assisted laser materials processing
Induction assisted laser materials processing Laser beam plus induction  The combined technologies overcome application barriers Issue The wide variety of potential applications of laser for welding and
More informationEffect of cooling rate on hardness and microstructure of AISI 1020, AISI 1040 and AISI 1060 Steels
International Journal of Physical Sciences Vol. 4 (9), pp. 514518, September, 2009 Available online at http://www.academicjournals.org/ijps ISSN 19921950 2009 Academic Journals Full Length Research Paper
More informationNorth American Stainless
North American Stainless Flat Products Stainless Steel Grade Sheet 310S (S31008)/ EN 1.4845 Introduction: SS310 is a highly alloyed austenitic stainless steel designed for elevatedtemperature service.
More information